The objective of this paper is to report a study on the prediction of the steadystate thermal resistance of woven compression bandage (WCB) by using three different mathematical models. The experimental samples of WCB were 100% cotton, cotton–polyamide–polyurethane, and viscose–polyurethane. The bandage samples were evaluated at extensions ranging at 10–100%, with two and threelayer bandaging techniques. Experimental thermal resistance was measured by thermal foot manikin (TFM) and ALAMBETA testing devices. The obtained results by TFM and ALAMBETA were validated and compared with the theoretical models (Maxwell–Eucken2, Schuhmeister, and Militky), and a reasonable correlation of approximately 78%, 92%, and 93% for ALAMBETA and 75%, 82%, and 83% for TFM, respectively, was observed.
Keywords
 Mathematical models for thermal resistance
 thermal foot manikin
 ALAMBETA
 woven bandage properties
Thermal manikins are devices by means of which it is possible to simulate heat exchange between humans and the environment [1, 2]. Human thermal comfort is defined as a condition of mind, which expresses satisfaction with the surrounding environment. High temperatures and humidity provide discomforting sensations and sometimes heat stress, which leads to reduce the body’s ability to cool itself. Moreover, this discomfort reduces the productivity of workers and may lead to more serious health problems, especially for aged people [3].
Clothing comfort is an important factor in the stage at which people make their clothing selections [3]. The thermal resistance (
The measurement of clothing insulation with a thermal manikin is a dynamically balanced adjustment process, which initially depends on the central temperature inside the manikin. It means that continuous adjustment of heat flux makes the manikin skin temperature approach a constant temperature gradually under the heat diffusion. These adjustments limit the change in the manikin skin temperature of all parts to a range of ±0.5°C around the required temperature. The final state is that the manikin skin temperature is steady and very close to the constant temperature [9].
The main factors affecting testing of
Convection is a process in which heat is transferred by a moving fluid (liquid or gas). For example, air in contact with the body is heated by conduction, and then carried away from the body by convection [13].
A common method for removing water from textiles is convective drying. When the fluid starts at a constant temperature and the surface temperature is suddenly increased above that of the fluid, there will be convective heat transfer from the surface to the fluid as a result of the temperature difference (Δ
When people wear multilayer clothing ensembles in cold weather conditions or in hot environments, air spaces are present between the skin and the inner layer or between two adjacent layers. The
The thermal resistance of fabrics can be calculated by means of experimental, analytical, and numerical methods [16, 17]. There are many models to be found within the textile engineering and heat transfer fields for the thermal resistance prediction. The preference of selection depends on the requisite precision and nature of the solution. Conductive heat transfer is the simplest way to illustrate mathematically and is often the key way of heat transfer [18].
Numerical solutions deal with materials of irregular shapes and properties, different types of heat transfer, and boundary conditions. Numerical methods also have the capability to achieve the maximum precision [19]. There are many commercially available softwares that allow users to solve their problems through numerical solutions. However, these methods are inherently more difficult and complicated, and in some conditions, simple methods prove to be more accurate at much less effort [20]. Thermal resistance is also predicted by using artificial neural networks and statistical models. Some researchers have predicted the thermal resistance of fabrics using mathematical approaches.
Schuhmeister suggested a relationship for the thermal conductivity prediction of fabrics by assuming onethird of fibers to be parallel and twothird in series with a homogeneous distribution in all directions [21]. Later, many researchers used Schuhmeister’s model by assuming different ratios of series and parallel components [22,23,24]. Presently, Mansoor et al. [25, 26] have modified Schuhmeister and Militky models by combining the water and fiber filling coefficients for the prediction of thermal resistance of wet socks.
Das et al. [27] calculated the heat transfer through the fabric assemblies with the electric resistance and Fricke’s law analogy by assuming them as cuboids packed with randomly oriented infinite fibers. Wie et al. [28] suggested a model for fabric thermal resistance prediction by assuming that heat passes through the fabric as a combination of fiber and air in series plus the air in parallel.
Most studies on
The Maxwell–Eucken (ME) model (Eq. (2)) can be used to describe the effective thermal conductivity of a twocomponent material with simple physical structures. In Eq. (2),
Schuhmeister summarized the relationship between the thermal conductivity and structural parameters of a fabric using Eq. (3):
Militky summarized the relationship between the thermal conductivity and structural parameters of a fabric using empirical Eq. (6) and used the same steps for calculating
It is assumed that fabric density changes with wetting, which causes a change in the filling coefficient, porosity, and thermal conductivity of the fabrics. Based on these assumptions the following three equations were developed that will be used to find the fabric density, filling coefficient, and thermal conductivity for different moisture levels. The average thermal conductivity for different fibers (within socks) at different moisture levels are calculated based on Eq. (7) as follows:
Filling coefficients for fiber and air are calculated as listed in Table 1, according to the following steps.
Filling coefficients calculation
Content  % 
Weight  G 
Area  m^{2} 
Areal density  g/m 
Volumetric density 

Filling coefficient 

Air filling coefficient (
The outputs of Eqs (7) and (8) are used as input for all the above models. Thermal conductivity of water and air is taken as 0.6 and 0.026 W/m/K while density of water is 1,000 Kg/m^{3}. The values of the different input parameters used in this study are listed in Table 2 [39].
Different fiber properties
Cotton  1,540  0.5 
Viscose  1,530  0.5 
Polyester  1,360  0.4 
Nylon 66  1,140  0.3 
Polypropylene  900  0.2 
Wool  1,310  0.5 
Acrylic  1,150  0.3 
Experimental samples are 100% bleached cotton (BLCO), cotton–polyamide–polyurethane (COPAPU), and viscose–polyurethane (VI–PU) bandages. All
Specifications of woven bandage samples on thermal foot manikin
Bleached cotton 100%  100% cotton, two layers, 50% extension, 50% overlap  Two layers = 212.3  One layer = 0.76 

Cotton 78%, polyamide 16%, polyurethane 6%  COPAPU, two layers, 50% extension, 50% overlap  Two layers = 238.1  One layer = 0.84 

Viscose 94%, polyurethane 6%  VIPU, two layers, 50% extension, 50% overlap  Two layers = 220.7  One layer = 0.79 

Bleached cotton 100%  100% cotton, three layers, 50% extension, 66% overlap  Three layers = 317.5  One layer = 0.76 

Cotton 78%, polyamide 16%, polyurethane 6%  COPAPU, three layers, 50% extension, 66% overlap  356.3  One layer = 0.84 

Viscose 94%, polyurethane 6%  VIPU, three layers, 50% extension, 66% overlap  329.4  One layer = 0.79 
Thermal manikins are designed to simulate the human body’s heat exchange and its interaction with the surrounding environment. There are two types of testing on thermal manikin, practically called “nude and clothed Manikin” [2]. Experimental samples consist of three types of WCBs, which as porous materials should provide thermal comfort to enable air permeability, heat transfer, and liquid perspiration out of the human body. Mercerized cotton socks were used to cover TFM as underwear to measure
However, the same tests were confirmed on ALAMBETA at the same extension and number of layers using special tensioning frame, as shown in Figure 3, but using the free air convection system [41].
The stabilization process of the TFM could be achieved after 20 min – at least – then the final testing step takes place [10].
Finally,
For comparison, all bandage types were wrapped on TFM and ALAMBETA at the same extension level ranging from 10% to 100% using both two and three layers of bandages [10]. Figure 5 illustrates that
The same analysis is proved for the three layers of bandages as demonstrated in Figures 6 and 8. Moreover, the effect of higher applied tension by threelayer bandaging appeared as the third main factor that decreases the volume of the air layers between the adjacent bandage layers.
The experimental results of
The transient heat flow is shown in Eq. (10), whereas the steadystate heat flow is shown in Eq. (11) as follows:
The experimental evaluation of
The obtained results of
Different fiber properties
Cotton  1,540  0.5 
Viscose  1,530  0.5 
Polyester  1,360  0.4 
Nylon 66  1,140  0.3 
Polypropylene  900  0.2 
Wool  1,310  0.5 
Acrylic  1,150  0.3 
Filling coefficients calculation
Content  % 
Weight  G 
Area  m^{2} 
Areal density  g/m 
Volumetric density 

Filling coefficient 

Specifications of woven bandage samples on thermal foot manikin
Bleached cotton 100%  100% cotton, two layers, 50% extension, 50% overlap  Two layers = 212.3  One layer = 0.76 

Cotton 78%, polyamide 16%, polyurethane 6%  COPAPU, two layers, 50% extension, 50% overlap  Two layers = 238.1  One layer = 0.84 

Viscose 94%, polyurethane 6%  VIPU, two layers, 50% extension, 50% overlap  Two layers = 220.7  One layer = 0.79 

Bleached cotton 100%  100% cotton, three layers, 50% extension, 66% overlap  Three layers = 317.5  One layer = 0.76 

Cotton 78%, polyamide 16%, polyurethane 6%  COPAPU, three layers, 50% extension, 66% overlap  356.3  One layer = 0.84 

Viscose 94%, polyurethane 6%  VIPU, three layers, 50% extension, 66% overlap  329.4  One layer = 0.79 
Automatic Identification Of Wrist Position In A Virtual Environment For Garment Design Pressure Evaluation Of Seamless Yoga Leggings Designed With Partition Structure Tensile Properties Analysis Of 3D FlatKnitted Inlay Fabric Reinforced Composites Using Acoustic Emission From Raw To Finished Cotton—Characterization By Interface Phenomena A Study on the Woven Construction of Fabric Dyed With Natural Indigo Dye and Finishing for Applying to Product Design for Home Textile Products A Calculation Method for the Deformation Behavior of WarpKnitted Fabric Nondestructive Test Technology Research for Yarn Linear Density Unevenness Blend Electrospinning of Poly(ƐCaprolactone) and Poly(Ethylene Glycol400) Nanofibers Loaded with Ibuprofen as a Potential Drug Delivery System for Wound Dressings Study On Structure And AntiUv Properties Of Sericin Cocoons Fit And Pressure Comfort Evaluation On A Virtual Prototype Of A TightFit Cycling Shirt A FabricBased Integrated Sensor Glove System Recognizing Hand Gesture Developing Real Avatars for the Apparel Industry and Analysing Fabric Draping in the Virtual Domain Review on Fabrication and Application of Regenerated Bombyx Mori Silk Fibroin MaterialsThe Effects of Sensory Marketing on ClothingBuying Behavior Transport of Moisture in Car Seat Covers Review on 3D Fabrication at Nanoscale Investigation of the Performance of Cotton/Polyester Blend in Different Yarn Structures Determination of Sewing Thread Consumption for 602, 605, and 607 Cover Stitches Using Geometrical and MultiLinear Regression Models Application of Spectral Analysis in Spinning Measurements Polyaniline Electrospun Composite Nanofibers Reinforced with Carbon Nanotubes Effect of Surface Modification of Himalayan Nettle Fiber and Characterization of the Morphology, Physical and Mechanical Properties Investigation of Actual Phenomena and Auxiliary Ultrasonic Welding Parameters on Seam Strength of PVCCoated Hybrid Textiles Modeling Lean and Six Sigma Integration using Deep Learning: Applied to a Clothing Company Comparative Analysis of Structure and Properties of Stereoscopic Cocoon and Flat Cocoon Effect of Different Yarn Combinations on Auxetic Properties of Plied Yarns Analysis of Heat Transfer through a Protective Clothing Package Smart Textile for Building and Living Investigation of Twist Waves Distribution along Structurally Nonuniform Yarn Preliminary Experimental Investigation of CutResistant Materials: A Biomimetic Perspective Durable WashResistant Antimicrobial Treatment of Knitted Fabrics Study on the Thermal and Impact Resistance Properties of Micro PA66/PU Synergistically Reinforced MultiLayered Biaxial Weft Knitted Fabric Composites FeaBased Structural Heat Transfer Characteristic of 3D Orthogonal Woven Composite Subjected to the NonUniform Heat Load ComfortRelated Properies of Cotton Seersucker Fabrics Investigating the Effect of Recycled Cotton Included Fabrics on the Thermal Behaviour by Using a Female Thermal Manikin Conductive Heat Transfer Prediction of Plain Socks in Wet State Textronic Solutions Used for Premature Babies: A Review Effect of Lycra Weight Percent and Loop Length on Thermophysiological Properties of Elastic Single Jersey Knitted Fabric Texture Representation and Application of Colored Spun Fabric Using Uniform ThreeStructure Descriptor Approach to Performance Rating of Retroreflective Textile Material Considering Production Technology and Reflector Size Influence of Multilayer Interlocked Fabrics Structure on their Thermal Performance Experimental Investigation of the Wettability of Protective Glove Materials: A Biomimetic Perspective Mechanical Properties of Composites Reinforced with Technical Embroidery Made of Flax Fibers Development of the Smart TShirt for Monitoring Thermal Status of Athletes Assessment and Semantic Categorization of Fabric Visual Texture Preferences Application of Coating Mixture Based on Silica Aerogel to Improve Thermal Protective Performance of Fabrics A Biomimetic Approach to Protective Glove Design: Inspirations from Nature and the Structural Limitations of Living Organisms Washing Characterization of Compression Socks Estimation of Seams in Paraglider Wing Development of a Small, Covered Yarn Prototype Numerical Prediction of the Heat Transfer in Air Gap of Different Garment Models Fabrication and Characterization of Fibrous Polycaprolactone Blended with Natural Green Tea Extracts Using Dual Solvent Systems Archaeology and Virtual Simulation Restoration of Costumes in the Han Xizai Banquet Painting Modeling of Material Characteristics of Conventional Synthetic Fabrics